The Influence of Hafnium Doping on Density of States in Zinc Oxide Thin-Film Transistors Deposited via Atomic Layer Deposition
© The Author(s). 2017
Received: 12 November 2016
Accepted: 17 January 2017
Published: 23 January 2017
The Erratum to this article has been published in Nanoscale Research Letters 2017 12:172
Thin-film transistors (TFTs) with atomic layer deposition (ALD) HfZnO (HZO) as channel layer and Al2O3 as gate insulator were successfully fabricated. Compared with ZnO-TFT, the stability of HZO-TFT was obviously improved as Hf doping can suppress the generation of oxygen related defects. The transfer characteristics of TFTs at different temperatures were also investigated, and temperature stability enhancement was observed for the TFT with Hf doping. The density of states (DOS) was calculated based on the experimentally obtained E a, which can explain the experimental observation. A high-field effect mobility of 9.4 cm2/Vs, a suitable turn-on voltage of 0.26 V, a high on/off ratio of over 107 and a steep sub-threshold swing of 0.3 V/decade were obtained in HZO-TFT. The results showed that temperature stability enhancement in HfZnO thin-film transistors are attributed to the smaller DOS.
ZnO-based thin-film transistors (TFT) have recently attracted a great deal of attention owing to their potential application in active matrix liquate crystal display (AMLCD) and active matrix organic light emitting diodes (AMOLED) [1–3]. As an important part of TFTs, channel layers play a crucial role in TFT performance. ZnO-based single channel layer or double channel layer, such as HZO , IGZO , and IZO/IGZO , has been investigated for use in TFTs because of their high mobility. Among those ZnO-based TFTs, amorphous indium-gallium-tin oxide (IGZO) TFTs are regarded as the most promising devices as indium and gallium have excellent lattice matching with ZnO and gallium could suppress carrier generation via oxygen vacancy formation in IGZO. Recently, LG Display has released a 55 in, full high-definition (FHD) OLED television which utilizes an IGZO TFT active matrix . However, materials such as indium (In) and gallium (Ga) have some disadvantages, including toxicity, element scarcity, and indium extraction in hydrogen plasma . Specifically, the instability of ZnO-based TFTs is still a problem hard to solve, as ZnO-based TFTs usually contain defects in the active channel layer and deep-level defects in the channel/insulator interface . To obtain highly stable Zn-based oxide TFTs, many studies have been devoted to the development of robust active layers by the incorporation of metal cations (such as Ga, Al, Hf, and Si) based on sputtering method or spin-coating method [10–14], with the expectation to reduce the density of defects such as oxygen vacancies. There are few reports on adopting ALD method to realize doping in Zn-based oxide TFTs. As it is known, ALD offers various advantages including accurate thickness and composition control, excellent uniformity and step coverage, low defect density, low deposition temperatures, and good reproducibility [15–17]. Furthermore, due to the self-limiting and layer-by-layer (or “digital”) growth, ALD exhibits the unique in situ atomic layer doping capability of achieving precise doping with atomic level control during the deposition process.
Up to now, to our limited knowledge, the deposition of channel layers using ALD has been focused on almost pure ZnO layers. Given its low standard electrode potential, Hf is a more efficient suppressor of the generation of oxygen vacancies. Adding Hf element could suppress the growth of columnar structure, and therefore drastically decrease the carrier concentration and hall mobility in HZO films [18–20]. Hence, in this paper, Hf doped ZnO has been deposited via ALD and applied in TFTs as channel layer. The related parameters such as the Hf contents, growth temperature, channel thickness, and width/length ratio (W = L) were evaluated and optimized. The influence of Hf doping on performance of ZnO-TFT was studied. Especially, the detailed effect of Hf doping on the DOS has never been addressed. In the present letter, the DOS was calculated based on the experimentally obtained E a, which can explain the experimental observation.
Results and Discussion
Comparison of the electrical properties of the devices
V on (V)
where V 0 = V GS−V th,0, V th,0 is the threshold voltage at the start of the stress measurement, β is the stretched exponential exponent, and τ reflects the characteristics of carrier trapping time. The obtained τ, β values are 1.58 × 106 s, 0.39 for ZnO-TFT, and 2.32 × 106 s, 0.56 for HZO-TFT, respectively. It demonstrates that the degradation of HZO-TFT is slower than that of ZnO-TFT under a long-time operation.
In summary, we have successfully fabricated HZO-TFT via ALD, and the effect of Hf-doped ZnO on the stability of device was studied. Significantly improved on/off ratio and temperature stress stability were obtained in the HZO-TFT due to the reduced DOS, to be specific, a high field-effect mobility of 9.4 cm2/Vs, a suitable turn-on voltage of 0.26 V, a high on/off ratio of over 107, a steep sub-threshold swing of 0.3 V/decade. The proposed HZO-TFT in this paper can act as driving devices in the next-generation flat panel displays.
This work is supported by the National Key Basic Research Program of China (2015CB655005), Science and Technology Commission of Shanghai Municipality Program (14DZ228090), Project of National Post-Doctor Fund (2015M580315) and National Natural Science Foundation of China (61077013, 61274082, 51072111, and 51302165).
XD carried out the experiments and drafted the manuscript. XD and JZ participated in the design of the study and performed the analysis. CQ, JS participated in the measurements. XJ conceived the study and participated in its design. JZ and ZZ supervised the overall study and polished the manuscript. All authors read and approved the final manuscript
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Nomura K, Ohta H, Takagi A, Kamiya T, Hosono H (2004) Room-temperature fabrication of transparent flexible thin-film transistors using amorphous oxide semiconductors. Nature (London) 432:488–492View ArticleGoogle Scholar
- Ji KH, Kim JI, Jung HY, Park SY, Mo YG, Jeong JH, Kwon JY, Ryu MK, Lee SY, Choi R, Jeong JK (2010) The effect of density-of-state on the temperature and gate bias-induced instability of InGaZnO thin film transistors. J Electrochem Soc 157:H983–H986View ArticleGoogle Scholar
- Namgung SD, Yang S, Park K, Cho A-J, Kim H, Kwon J-Y (2015) Influence of post-annealing on the off current of MoS2 field-effect transistors. Nanoscale Res Lett 10:62View ArticleGoogle Scholar
- Wu J, Han DD, Cong YY, Zhao NN, Chen ZF, Dong JC, Zhao FL, Zhang SD, Liu LF, Zhang X, Wang Y (2015) Effects of channel thickness on characteristics of HZO-TFTs fabricated at low temperature. Electron Lett 51:867–869View ArticleGoogle Scholar
- Nomura K, Ohta H, Ueda K, Kamiya T, Hirano M, Hosono H (2003) Thin-film transistor fabricated in single-crystalline transparent oxide semiconductor. Science 300:1269–1272Google Scholar
- Ding X, Zhang H, Ding H, Zhang J, Huang C, Shi W, Li J, Jiang X, Zhang Z (2014) Growth of IZO/IGZO dual-active-layer for low-voltage-drive and high-mobility thin film transistors based on an ALD grown Al2O3 gate insulator. Superlattice Microst 76:156–162View ArticleGoogle Scholar
- Han CW, Kim KM, Bae SJ, Choi HS, Lee JM, Kim TS, Tak YH, Cha SY, Ahn BC (2012) 21.2: 55-inch FHD OLED TV employing New Tandem WOLEDs. SID Int Symp Dig Tech Pap 43:279–281View ArticleGoogle Scholar
- Rim YS, Kim SM, Kim KH (2008) Effects of substrate heating and film thickness on properties of silver-based ZnO multilayer thin films. Jpn J Appl Phys 47:5022–5027View ArticleGoogle Scholar
- Han DS, Park JH, Kang YJ, Park JW (2013) Improvement in the bias stability of zinc-tin oxide thin-film transistors by hafnium doping. J Electron Mater 42:2470–2477View ArticleGoogle Scholar
- Kim C-J, Kim S, Lee J-H, Park J-S, Kim S, Park J, Lee E, Lee J, Park Y, Kim JH, Shin ST, Chung U-I (2009) Amorphous hafnium-indium-zinc oxide semiconductor thin film transistors. Appl Phys Lett 95:252103View ArticleGoogle Scholar
- Chong E, Jo KC, Lee SY (2010) High stability of amorphous hafnium-indium-zinc-oxide thin film transistor. Appl Phys Lett 96:152102View ArticleGoogle Scholar
- Ahn CH, Yun MG, Lee SY, Cho HK (2014) Enhancement of electrical stability in oxide thin-film transistors using multilayer channels grown by atomic layer deposition. IEEE T Electron Dev 61:73–78View ArticleGoogle Scholar
- Hosono H (2006) Ionic amorphous oxide semiconductors: Material design, carrier transport, and device application. J Non-Cryst Solids 352:851–858View ArticleGoogle Scholar
- Ahn CH, Kong BH, Kim H, Cho HK (2011) Improved electrical stability in the Al doped ZnO thin-film-transistors grown by atomic layer deposition. J Electrochem Soc 158:H170–H173View ArticleGoogle Scholar
- Shih H-Y, Chu F-C, Das A, Lee C-Y, Chen M-J, Lin R-M (2016) Atomic layer deposition of gallium oxide films as gate dielectrics in AlGaN/GaN metal-oxide-semiconductor high-electron-mobility transistors. Nanoscale Res Lett 11:1–9View ArticleGoogle Scholar
- Zheng L-L, Ma Q, Wang Y-H, Liu W-J, Ding S-J, Zhang DW (2016) High-Performance unannealed a-InGaZnO TFT with an Atomic-Layer-Deposited SiO2 insulator. IEEE Electr Device L 37:743–746Google Scholar
- Puurunen RL (2005) Surface chemistry of atomic layer deposition: a case study for the trimethylaluminum/water process. J Appl Phys 97:121301View ArticleGoogle Scholar
- Park J-S, Kim H, Kim I-D (2014) Overview of electroceramic materials for oxide semiconductor thin film transistors. J Electroceram 32:117–140View ArticleGoogle Scholar
- Park JS, Maeng W-J, Kim H-S, Park J-S (2012) Review of recent developments in amorphous oxide semiconductor thin-film transistor devices. Thin Solid Films 520:1679–1693View ArticleGoogle Scholar
- Kim C-J, Kim S, Lee J-H, Park J-S, Kim S, Park J, Lee E, Lee J, Park Y, Kim JH, Shin ST, Chung U-I (2009) Amorphous hafnium-indium-zinc oxide semiconductor thin film transistors. Appl Phys Lett 95:252103Google Scholar
- Kim W-S, Moon Y-K, Kim K-T, Shin S-Y, Ahn BD, Lee J-H, Park J-W (2011) The influence of hafnium doping on bias stability in zinc oxide thin film transistors. Thin Solid Films 519:5161–5164View ArticleGoogle Scholar
- Li C-H, Chen J-Z, Cheng I-C (2013) Transitions of bandgap and built-in stress for sputtered HfZnO thin films after thermal treatments. J Appl Phys 114:084503View ArticleGoogle Scholar
- Li C-H, Chen J-Z (2014) Electrical, optical, and microstructural properties of sol–gel derived HfZnO thin films. J Alloy Compd 601:223–230View ArticleGoogle Scholar
- Kim W-S, Moon Y-K, Kim K-T, Shin S-Y, Ahn BD, Lee J-H, Park J-W (2011) Improvement in the negative bias temperature stability of ZnO based thin film transistors by Hf and Sn doping. Thin Solid Films 519:6849–6852View ArticleGoogle Scholar
- Kim W-S, Moon Y-K, Kim K-T, Shin S-Y, Ahn BD, Lee J-H, Park J-W (2010) The influence of the hafnium doping on negative bias stability in zinc oxide thin film transistor. Electrochem Solid-State Lett 13:H295–H297View ArticleGoogle Scholar
- Kim Y-S, Park CH (2009) Rich variety of defects in ZnO via an attractive interaction between O vacancies and Zn interstitials: origin of n-type doping. Phys Rev Lett 102:086403View ArticleGoogle Scholar
- Kofstad P (1962) Studies of electrical conductivity of Nb2O5 as a function of oxygen pressure at 600–1200°C. J Phys Chem Solids 23:1571–1578View ArticleGoogle Scholar
- Gavryushin V, Raˇciukaitis G, Juodžbalis D, Kazlauskas A, Kubertaviˇcius V (1994) Characterization of intrinsic and impurity deep levels in ZnSe and ZnO crystals by nonlinear spectroscopy. J Cryst Growth 138:924–933View ArticleGoogle Scholar
- Takechi K, Nakata M, Eguchi T, Yamaguchi H, Kaneko S (2009) Comparison of ultraviolet photo-field effects between hydrogenated amorphous silicon and amorphous InGaZnO4 thin-film transistors. J Appl Phys 48:011301View ArticleGoogle Scholar
- Gavryushin V, Raciukaitis G, Juodzbalis D, Kazlauskas A, Kubertavicius V (1994) Characterization of intrinsic and impurity deep levels in ZnSe and ZnO crystals by nonlinear spectroscopy. J Cryst Growth 138:924–933View ArticleGoogle Scholar
- Indluru A, Alford TL (2010) High-temperature stability and enhanced performance of a-Si: H TFT on flexible substrate due to improved interface quality. IEEE T Electron Dev 57:3006–3011View ArticleGoogle Scholar
- Pichon L, Mercha A, Carin R, Bonnaud O, Mohammed-Brahim T, Helen Y, Rogel R (2000) Analysis of the activation energy of the subthreshold current in laser-and solid-phase-crystallized polycrystalline silicon thin-film transistors. Appl Phys Lett 77:576View ArticleGoogle Scholar
- Tai YH, Chiu HL, Chou LS (2012) The deterioration of a-IGZO TFTs owing to the copper diffusion after the process of the source/drain metal formation. J Electrochem Soc 159:J200–J203View ArticleGoogle Scholar
- Jeong JK, Yang S, Cho D-H, Park S-HK, Hwang C-S, Cho KI (2009) Impact of device configuration on the temperature instability of Al–Zn–Sn–O thin film transistors. Appl Phys Lett 95:123505View ArticleGoogle Scholar
- Chang G-W, Chang T-C, Jhu J-C, Tsai T-M, Syu Y-E, Chang K-C, Jian F-Y, Hung Y-C, Tai Y-H (2013) N2O plasma treatment suppressed temperature-dependent sub-threshold leakage current of amorphous indium–gallium–zinc-oxide thin film transistors. Surf Coat Tech 231:281–284View ArticleGoogle Scholar
- Lee JM, Cho IT, Lee JH, Kwon HI (2008) Bias-stress-induced stretched-exponential time dependence of threshold voltage shift in InGaZnO thin film transistors. Appl Phys Lett 93:093504View ArticleGoogle Scholar